Rhenium

75

tungsten ← rhenium → osmium


Tc
↑
Re
↓
Bh




periodic table




General


Name, Symbol, Number

rhenium, Re, 75


Chemical series
transition metals


Group, Period, Block

7, 6, d


Appearance
grayish white 



Atomic mass
186.207(1) g/mol


Electron configuration
[Xe] 4f14 5d5 6s2


Electrons per shell
2, 8, 18, 32, 13, 2


Physical properties


Phase
solid


Density (near r.t.)
21.02 g/cm³


Liquid density at m.p.
18.9 g/cm³


Melting point
3459 K
(3186 °C, 5767 °F)


Boiling point
5869 K
(5596 °C, 10105 °F)


Heat of fusion
60.43 kJ/mol


Heat of vaporization
704 kJ/mol


Heat capacity
(25 °C) 25.48 J/(mol·K)




Vapor pressure


P/Pa
1
10
100
1 k
10 k
100 k


at T/K
3303
3614
4009
4500
5127
5954



Atomic properties


Crystal structure
hexagonal


Oxidation states
7, 6, 4, 2, −2
(mildly acidic oxide)


Electronegativity
1.9 (Pauling scale)


Ionization energies
(more)

1st: 760 kJ/mol


2nd: 1260 kJ/mol


3rd: 2510 kJ/mol


Atomic radius
135 pm


Atomic radius (calc.)
188 pm


Covalent radius
159 pm


Miscellaneous


Magnetic ordering
?


Electrical resistivity
(20 °C) 193 nΩ·m


Thermal conductivity
(300 K) 48.0 W/(m·K)


Thermal expansion
(25 °C) 6.2 µm/(m·K)


Speed of sound (thin rod)
(20 °C) 4700 m/s


Speed of sound (thin rod)
(r.t.) 463 m/s


Shear modulus
178 GPa


Bulk modulus
370 GPa


Poisson ratio
0.30


Mohs hardness
7.0


Vickers hardness
2450 MPa


Brinell hardness
1320 MPa


CAS registry number
7440-15-5


Notable isotopes




Main article: Isotopes of rhenium


iso

NA

half-life

DM

DE (MeV)

DP


185Re

37.4%

Re is stable with 110 neutrons


187Re

62.6%

4.35×1010 y

α

1.653

183Ta


β-

0.003

187Os


Rhenium (chemical symbol Re, atomic number 75) is a silvery-white, lustrous, rare metal. Obtained as a byproduct of molybdenum refinement, it is among the ten most expensive metals on Earth. It is extremely resistant to wear and has one of the highest melting points of all elements. Its alloys with molybdenum or tungsten are superconducting. In combination with platinum, it makes good catalysts for the preparation of high-octane gasoline. It is also a component of high-temperature superalloys for jet engine parts.

Contents

1 Occurrence
2 History
3 Notable characteristics

3.1 Isotopes


4 Compounds
5 Applications
6 Precautions
7 See also
8 Footnotes
9 References
10 External links
11 Credits



Occurrence
Rhenium is widely spread in the Earth's crust, at approximately 0.001 parts per million (ppm), but it is not found free in nature. Some molybdenum ores contain 0.002 percent to 0.2 percent rhenium. It was only recently that the first rhenium mineral was found. In 1994, Nature published a letter describing a rhenium sulfide mineral found condensing from a fumarole on Russia's Kudriavy volcano.[1] This mineral, however, is not an economically viable source of the element.
Commercial rhenium is extracted from molybdenum roaster-flue dusts obtained from copper sulfide ores. Total world production is between 40 and 50 tons/year; the main producers are Chile, the United States, and Kazakhstan. Recycling of used platinum-rhenium catalyst and special alloys allow the recovery of another ten tons/year.

History
The name rhenium is derived from the Latin word Rhenus, meaning "Rhine." Before this element was discovered, its existence was predicted by Henry Moseley in 1914, based on his examination of the periodic table. Its discovery is generally attributed to Walter Noddack, Ida Tacke, and Otto Berg in Germany. In 1925, they reported detecting the element in platinum ore and in the mineral columbite. They also found rhenium in gadolinite and molybdenite. In 1928, they succeeded in extracting one gram (g) of the element by processing 660 kilograms (kg) of molybdenite.
The process was so complicated and the cost so high that production was discontinued until early 1950, when tungsten-rhenium and molybdenum-rhenium alloys were prepared. These alloys found important applications in industry, resulting in a high demand for rhenium produced from the molybdenite fraction of porphyry copper ores.

Notable characteristics
Rhenium is classified as a transition metal. In the periodic table, it lies in group seven (former group 7B), below manganese and technetium. It thus resembles the latter two elements in chemical properties. In addition, rhenium is situated in period six, between tungsten and osmium.
The melting point of rhenium is among the highest of all elements, exceeded only by the melting points of tungsten and carbon. Rhenium is also one of the densest, exceeded only by the densities of platinum, iridium, and osmium. The oxidation states of rhenium include -3,-1,+1,+2,+3,+4,+5,+6 and +7. Of these, the most common are +7,+6,+4,+2 and -1.
The usual commercial form of rhenium is a powder, but it can be consolidated by pressing and resistance-sintering in a vacuum or hydrogen atmosphere. This procedure yields a compact shape that is more than 90 percent of the density of the metal. When annealed, this metal is very ductile and can be bent, coiled, or rolled. Rhenium-molybdenum alloys are superconductive at ten Kelvin (K), and tungsten-rhenium alloys are superconductive around four to eight K, depending on the alloy.[2]

Isotopes
Naturally occurring rhenium is a mix of 185Re, which is stable, and 187Re, which is radioactive but has a very long half-life. Many other radioactive isotopes are known, with atomic mass numbers ranging from 160 to 194, but most of them are extremely short-lived.

Compounds
Ammonium perrhenate (APR, NH4ReO4): This salt of rhenium is the most common form in which rhenium is traded. Its rhenium content is around 69.0–69.4 percent. Pure rhenium powder can be produced from APR simply by reducing the latter with hydrogen.
Perrhenic acid (HReO4): This is a strong acid that can attack metals, metal oxides, carbonates, and hydroxides. It is, however, non-oxidizing. It exists only in solution—the solid has not been isolated. It is a common precursor to other rhenium compounds, some of have applications in the petrochemical and fine chemical industries.
Rhenium trioxide or rhenium (VI) oxide (ReO3): This oxide is a red solid with a metallic luster. It is the only stable trioxide of the Group seven elements (manganese, technetium, rhenium). It can be formed by reducing rhenium (VII) oxide (Re2O7) with carbon monoxide. Unlike most oxides, it exhibits very low resistivity. Instead, it behaves more like a metal in that its resistivity decreases as its temperature is lowered. In crystals of the oxide, each rhenium atom is surrounded by six oxygen atoms, forming a ReO6 octahedron.
Applications
Rhenium is combined with platinum to form catalysts that are used primarily for making lead-free, high-octane gasoline. It is also a component of high-temperature superalloys that are used to make jet engine parts. Additional uses of rhenium are given below.

It is widely used for filaments in mass spectrographs and ion gauges.
As an additive in tungsten and molybdenum-based alloys, it increases their ductility.
Catalysts made with rhenium are very resistant to chemical poisoning and are used in certain types of hydrogenation reactions.
Based on its good wear resistance and ability to withstand arc corrosion, rhenium is used in electrical contact material.
Thermocouples containing alloys of rhenium and tungsten are used to measure temperatures up to 2200 °C.
Rhenium wire is used in photoflash lamps in photography.
Precautions
Little is known about the toxicity of rhenium, but as a precautionary measure, it should be handled with care.

See also
Chemical element
Metal
Periodic table
Transition metal
Footnotes

↑ Korzhinsky, M.A. and S. I. Tkachenko, K. I. Shmulovich, Y. A. Taran and G. S. Steinberg (2004-05-05). Discovery of a pure rhenium mineral at Kudriavy volcano. Nature 369: 51–­­­52.

↑ The Superconductivity of Some Intermetallic Compounds Retrieved December 4, 2007.


ReferencesISBN links support NWE through referral fees
Chang, Raymond. 2006. Chemistry, 9th ed. New York: McGraw-Hill Science/Engineering/Math. ISBN 0073221031
Cotton, F. Albert and Geoffrey Wilkinson. 1980. Advanced Inorganic Chemistry, 4th ed. New York: Wiley. ISBN 0-471-02775-8
Greenwood, N.N. and Earnshaw, A. 1998. Chemistry of the Elements, 2nd Edition. Oxford, U.K.; Burlington, Massachusetts: Butterworth-Heinemann, Elsevier Science. ISBN 0750633654
Rhenium Los Alamos National Laboratory. Retrieved December 4, 2007.
External links
All links retrieved December 8, 2022.

WebElements.com - Rhenium

Credits
New World Encyclopedia writers and editors rewrote and completed the Wikipedia article
in accordance with New World Encyclopedia standards. This article abides by terms of the Creative Commons CC-by-sa 3.0 License (CC-by-sa), which may be used and disseminated with proper attribution. Credit is due under the terms of this license that can reference both the New World Encyclopedia contributors and the selfless volunteer contributors of the Wikimedia Foundation. To cite this article click here for a list of acceptable citing formats.The history of earlier contributions by wikipedians is accessible to researchers here:

Rhenium  history
Ammonium_perrhenate  history
Perrhenic_acid  history
Rhenium_trioxide  history
The history of this article since it was imported to New World Encyclopedia:

History of "Rhenium"
Note: Some restrictions may apply to use of individual images which are separately licensed.